Download presentation

Presentation is loading. Please wait.

Published byJeffery Pepin Modified over 2 years ago

2
Lecture #13 Properties of Hardening Concrete

3
Curing

4
Cracking Factors

5
Temperature and Evaporation

6
Thermal Stress Temperature change Coefficient of thermal expansion Concrete stiffness Cracking stress

7
Concrete Thermal Contraction = = Coefficient of thermal expansion ~ 5*10-6 / o F = Difference in concrete temperature (T) and the concrete setting temperature (T set ) = T set - T T= Variation of the average concrete temperature after placement. Assume this variation tracks closely to the 24-hour ambient air temperature cycle (after a 72 hour period). T set = 0.95(T conc + T H )

8
Concrete Thermal Contraction (con’t) T conc = Concrete placement temperature at construction ( o F). Assume this value (approx. 80 o F) = Change in concrete temperature due to heat of hydration = H u = Total heat of hydration per gram (kJ/g) = 0.007 (T conc ) – 3x10 -5 (T conc ) 2 –0.0787 C= amount of cement (grams) per m 3 = Degree of hydration (estimate to be approximately 0.15-0.2) c p = Specific heat of cement = 1.044 kJ/g = Density of concrete ~ 2400 kg/m 3

10
Strength(f t ) vs. Time f t = a log (t) + b

11
TEMPERATURE (C) 40 30 20 10 0 -10 -20 0 12 24 36 48 60 72 84 96 TIME (hours) FIGURE 1. The Nurse-Saul Maturity Function

12
S M, t e

13
Maturity

14
Maturity Concepts Nurse - Saul Equation (units: Temp – Time) Maturity: Product of time & temperature T o = Datum Temperature T = Average Concrete Temperature over Time “t” M = Maturity

15
ARRHENIUS EQUATIONS E = Activation Energy R = Gas Constant t e = Equivalent Age or Time

16
LABORATORY TESTING FIELD MEASUREMENT Procedures for using maturity method involve laboratory testing and field measurements.

17
Elastic Modulus

18
Sawcut Timing and Depth

19
Curing

20
Strength Factors

21
Relative Humidity at ¾ inch

22
Effective Curing Thickness Effective Curing Thickness

23
Curing Quality Wind No Wind

24
Model of CSH Structure of CSH

25
Nature of Concrete Creep and Shrinkage

26
Typical creep curve for cement paste. a Microstrain Time after loading Creep strain Elastic recovery Creep recovery Irreversible creep Concrete unloaded Elastic strain

27
Burger Model Constant Stress (Creep) time Strain

28
Creep of cement under simultaneous loading & drying. 62 sh =free shrinkage; bc =basic creep (specimen loaded but not drying); dc =drying creep; cr =total creep strain; tot =total strain (simultaneous loading & drying) b Free shrinkage (no load) Basic creep (no drying) Loading and drying Microstrain Time sh bc dc cr tot

29
Spring-Loaded Creep Frame CCCCCCCCCC 6 X 3 IN. PLUG (CONCRETE) C = 6 X 12 IN. TEST CYLINDERS 6 X 3 IN. PLUG (CONCRETE) UPPER JACK PLATE LOAD BARS LOWER JACK PLATE UPPER LOAD PLATE LOWER LOAD PLATE UPPER BASE PLATE SPRINGS LOWER BASE PLATE

30
Horizontal Mold for Creep Specimens

31
Cracking Frame

32
The Cracking Frame Test specimen strain gauge T = 1.0 10 -6 K -1 T = 12 10 -6 K -1

33
Crack in Specimen

34
Preparation of Fracture Specimens

35
Determination of Creep where crp = Creep strain v = Shrinkage strain (ASTM C 157) e = Frame strain F s = Force in concrete (F) E c = Modulus of elasticity of concrete (F/L -2 ) A c = Specimen cross sectional area (L 2 )

36
Accumulative vs. Time

37
Burger Model Constant Stress (Creep) time Strain

38
Aggregate Effects

39
Effects of Paste Properties Effect of age of loading on the creep strain. Effect of w/c ratio on the shrinkage strain.

40
Mechanisms of Creep and Shrinkage Creep It is a complex process involving slipping of surfaces past one another within the structure of C-S-H. It is a function of pore structure and ease of slippage of C-S-H particles. As the space between particles becomes less and less the degree of creep becomes less and less. Drying Shrinkage Moisture loss is driven by the ambient relative humidity. As moisture escapes from the capillaries, menisci are created and capillary stresses are developed. As more moisture is evaporated, smaller and smaller menisci are created. This action creates stress and causes slippage between C-S-H particles.

41
This method is based upon a method proposed by Branson and Christiason (2.3) and was developed by ACI Committee 209 (2.4) In 1982, ACI Special Publication 76 (2.5) gives an updated but not significantly changed version of this method. This method uses the as the creep coefficient. ACI Committee 209 Method

42
Shrinkage – ACI The shrinkage strain at t days after the end of initial curing is where = ultimate shrinkage strain = 415 to 1070 micro-strain = 0.9 to 1.10 and f = 20 to 130 days In the absence of specific data for local aggregate and conditions Committee 209 suggests that With = product of applicable correction factors The equations for the correction factors are given in Table A

43
The creep coefficient at t days after loading is given by where = ultimate creep coefficient = 1.30 to 4.15 = 0.40 to 0.80 d = 6 to 30 days In the absence of specific data for local aggregates and conditions Committee 209 suggests that where = product of applicable correction factors The equations for the correction factors are given in Table A Creep – ACI 209

44
The concrete strength at t days is given by with suggested values of a = 4.0 days = 0.85 for most cured ordinary Portland cement concrete. The modulus of elasticity E c at t days is given by which is often taken as when E and f’ c are in MPa Strength and Modulus of Elasticity

45
NotesCorrection Factors CreepShrinkage Loading Age Relative Humidity Average h=average 1.14 - 0.00092 h 1.23 - 0.0015 h during 1st year Thicknessthickness in mm for 1st yr. of 150 < h < 300 loading 1.10 - 0.00067 h 1.17 - 0.0014 h ultimate value ultimate value Concrete s= slump in mm 0.82 + 0.00264s 0.89 +.00161s Composition c= cement content - kg/m 3 0.75 +.00061c Table A ACI Creep and Shrinkage Correction Factors

Similar presentations

Presentation is loading. Please wait....

OK

Engineering Properties of Wood

Engineering Properties of Wood

© 2017 SlidePlayer.com Inc.

All rights reserved.

Ads by Google

Ppt on campus recruitment systems Ppt on zener diode voltage Best ppt on geothermal energy Ppt on holographic technology video Ppt on email etiquettes presentation pro Ppt on different forms of power sharing Ppt on case study of drought in india Ppt on breast cancer awareness Ppt on rainy season in india Ppt on global warming with pictures